* Measurement of the emissivities of gases at temperatures up to 1000 °C. Emissivity values were required for gaseous aluminium chlorides as part of the development of the sub-halide distillation process mentioned above. A flowing column of the gas to be measured, heated in a refractory tube, was maintained at a fixed length by gas barriers at each end, formed by balanced opposing streams of argon.  The radiation emitted by the gas was measured by a thermopile. A diaphragm was set up to shield this sensor from radiation emitted by the furnace and other hot parts of the equipment.  The whole apparatus was mounted on a water-cooled optical bench.
* X-ray diffraction determination of the structures of liquid metals. There was a need for structural studies of liquid sodium and sodium-potassium alloys because these were used as coolants in fast-breeder reactors.  Fulmer developed a high temperature x-ray diffractometer for investigating the structures of liquid metals and alloys. In addition to its studies of liquid alkali metals, Fulmer discovered that certain eutectics, such as those in the gold-silicon and gold-germanium systems, have a structure in the liquid phase that has to be disrupted on crystallization.  This gives rise to considerable supercooling which results in multiple nucleation, and hence a very fine grain size in the resulting polycrystalline alloy.
* Production of high purity austenitic stainless steel. High purity austenitic stainless steel was of interest as a potential cladding material for nuclear fuel elements. Fulmer produced high purity chromium by electro-deposition from a fluoride bath. Zone refining using induction heating was used to produce high-purity iron and nickel and to remove oxygen from chromium. Impurity levels of 1-40 parts per million were achieved.
* Chromium with improved ductility. Uses of chromium as a high temperature material are limited by its brittleness.  Starting with electro-deposited flakes of high purity chromium, investigators at Fulmer used argon-arc melting to form electrodes for ingot production in a consumable electrode furnace. Ingots were then heated in an inert or hydrogen atmosphere and extruded to give a fine grained structure.  Critical warm working, below the recrystallization temperature, then gave improved room-temperature ductility.
* Statistical studies of the strength of ceramics. The strength of brittle materials such as ceramics is inherently variable. Fulmer undertook numerous strength tests on sets of nominally identical specimens of engineering ceramics such as silicon nitride and silicon carbide.  They devised graphical techniques for finding the probability distribution of test results and contributed to criteria for engineering design with these materials.